Experimental and theoretical studies of nanofluid thermal conductivity enhancement: a review
 Clement Kleinstreuer^{1}Email author and
 Yu Feng^{1}
DOI: 10.1186/1556276X6229
© Kleinstreuer and Feng; licensee Springer. 2011
Received: 1 October 2010
Accepted: 16 March 2011
Published: 16 March 2011
Abstract
Nanofluids, i.e., welldispersed (metallic) nanoparticles at low volume fractions in liquids, may enhance the mixture's thermal conductivity, k_{nf}, over the basefluid values. Thus, they are potentially useful for advanced cooling of microsystems. Focusing mainly on dilute suspensions of welldispersed spherical nanoparticles in water or ethylene glycol, recent experimental observations, associated measurement techniques, and new theories as well as useful correlations have been reviewed.
It is evident that key questions still linger concerning the best nanoparticleandliquid pairing and conditioning, reliable measurements of achievable k_{nf} values, and easytouse, physically sound computer models which fully describe the particle dynamics and heat transfer of nanofluids. At present, experimental data and measurement methods are lacking consistency. In fact, debates on whether the anomalous enhancement is real or not endure, as well as discussions on what are repeatable correlations between k_{nf} and temperature, nanoparticle size/shape, and aggregation state. Clearly, benchmark experiments are needed, using the same nanofluids subject to different measurement methods. Such outcomes would validate new, minimally intrusive techniques and verify the reproducibility of experimental results. Dynamic k_{nf} models, assuming noninteracting metallic nanospheres, postulate an enhancement above the classical Maxwell theory and thereby provide potentially additional physical insight. Clearly, it will be necessary to consider not only one possible mechanism but combine several mechanisms and compare predictive results to new benchmark experimental data sets.
Introduction
A nanofluid is a dilute suspension of nanometersize particles and fibers dispersed in a liquid. As a result, when compared to the base fluid, changes in physical properties of such mixtures occur, e.g., viscosity, density, and thermal conductivity. Of all the physical properties of nanofluids, the thermal conductivity (k_{nf}) is the most complex and for many applications the most important one. Interestingly, experimental findings have been controversial and theories do not fully explain the mechanisms of elevated thermal conductivity. In this paper, experimental and theoretical studies are reviewed for nanofluid thermal conductivity and convection heat transfer enhancement. Specifically, comparisons between thermal measurement techniques (e.g., transient hotwire (THW) method) and optical measurement techniques (e.g., forced Rayleigh scattering (FRS) method) are discussed. Recent theoretical models for nanofluid thermal conductivity are presented and compared, including the authors' model assuming welldispersed spherical nanoparticles subject to micromixing effects due to Brownian motion. Concerning theories/correlations which try to explain thermal conductivity enhancement for all nanofluids, not a single model can predict a wide range of experimental data. However, many experimental data sets may fit between the lower and upper meanfield bounds originally proposed by Maxwell where the static nanoparticle configurations may range from a dispersed phase to a pseudocontinuous phase. Dynamic k_{nf} models, assuming noninteracting metallic nanospheres, postulate an enhancement above the classical Maxwell theory and thereby provide potentially additional physical insight. Clearly, it will be necessary to consider not only one possible mechanism but combine several mechanisms and compare predictive results to new benchmark experimental data sets.
Experimental studies
Nanofluids are a new class of heat transfer fluids by dispersing nanometersize particles, e.g., metaloxide spheres or carbon nanotubes, with typical diameter scales of 1 to 100 nm in traditional heat transfer fluids. Such colloidal dispersions may be uniform or somewhat aggregated. Earlier experimental studies reported greater enhancement of thermal conductivity, k_{nf}, than predicted by the classical model of Maxwell [1], known as the meanfield or effective medium theory. For example, Masuda [2] showed that different nanofluids (i.e., Al_{2}O_{3}water, SiO_{2}water, and TiO_{2}water combinations) generated a k_{nf} increase of up to 30% at volume fractions of less than 4.3%. Such an enhancement phenomenon was also reported by Eastman and Choi [3] for CuOwater, Al_{2}O_{3}water and CuOil nanofluids, using the THW method. In the following decades, it was established that nanofluid thermal conductivity is a function of several parameters [4, 5], i.e., nanoparticle material, volume fraction, spatial distribution, size, and shape, as well as basefluid type, temperature, and pH value. In contrast, other experimentalists [6–9], reported that no correlation was observed between k_{nf} and nanofluid temperature T. Furthermore, no k_{nf} enhancement above predictions based on Maxwell's effective medium theory for noninteracting spherical nanoparticles was obtained [5]. Clearly, this poses the question if nanofluids can provide greater heat transfer performance, as it would be most desirable for cooling of microsystems. Some scientists argued that the anomalous k_{nf} enhancement data are caused by inaccuracies of thermal measurement methods, i.e., mainly intrusive vs. nonintrusive techniques. However, some researchers [10, 11], relying on both optical and thermal measurements, reported k_{nf} enhancements well above classical model predictions. When comparing different measurement methods, error sources may result from the preparation of nanofluids, heating process, measurement process, cleanliness of apparatus, and if the nanoparticles stay uniformly dispersed in the base fluid or aggregate [12]. Thus, the controversy is still not over because of those uncertainties.
Experimental measurement methods
Transient hotwire method
THW method is the most widely used static, linear source experimental technique for measuring the thermal conductivity of fluids. A hot wire is placed in the fluid, which functions as both a heat source and a thermometer [20, 21]. Based on Fourier's law, when heating the wire, a higher thermal conductivity of the fluid corresponds to a lower temperature rise. Das [22] claimed that during the short measurement interval of 2 to 8 s, natural convection will not influence the accuracy of the results.
For the experimental procedure, the wire is heated via a constant electric power supply at step time t. A temperature increase of the wire is determined from its change in resistance which can be measured in time using a Wheatstonebridge circuit. Then the thermal conductivity is determined from Eq. 4, knowing the heating power (or heat flux q) and the slope of the curve ln(t) versus T.
The advantages of THW method are low cost and easy implementation. However, the assumptions of an infinite wirelength and the ambient acting like a reservoir (see Eqs. 1 and 2c) may introduce errors. In addition, nanoparticle interactions, sedimentation and/or aggregation as well as natural convection during extended measurement times may also increase experimental uncertainties [19, 23].
Other thermal measurement methods
A number of improved hotwire methods and experimental designs have been proposed. For example, Zhang [24] used a shorthotwire method (see also Woodfield [25]) which can take into account boundary effects. Mintsa [26] inserted a mixer into his THW experimental devices in order to avoid nanoparticle aggregation/deposition in the suspensions. Ali et al. [27] combined a laser beam displacement method with the THW method to separate the detector and heater to avoid interference.
Alternative static experimental methods include the temperature oscillation method [16, 17, 28], microhotstrip method [29], steadystate cutbar method [30], 3ω method [18, 31, 32], radial heatflow method [33], photothermal radiometry method [34], and thermal comparator method [19, 35].
Summary of experimental studies on convective heat transfer properties of nanofluids
Reference  Nanofluids  Flow nature  Findings 

Pak and Cho [91]  d_{p} = 13 nm spherical Al_{2}O_{3}water d_{p} = 27 nm spherical TiO_{2}water  Tube/turbulent  Nu is 30% larger than conventional base fluid and larger than DittusBoelter prediction 
Li and Xuan [92]  d_{p} < 100 nm spherical Cuwater  Tube/turbulent  Nu is larger than DittusBoelter prediction when volume fraction φ > 0.5% 
Wen and Ding [93]  d_{p} = 2756 nm spherical Al_{2}O_{3}water  Tube/laminar  Nu > 4.36 for fullydeveloped pipe flow with constant wall heat flux 
Ding [94]  d_{p} > 100 nm rodlike carbon nanotubewater  Tube/laminar  Nu increase more than 300% at Re = 800 
Heris [95]  d_{p} = 20 nm spherical Al_{2}O_{3}water  Tube/laminar  Nu measured is larger than Nu of pure water 
Williams [49]  d_{p} = 46 nm spherical Al_{2}O_{3}water d_{p} = 60 nm spherical ZrO_{2}water  Tube/turbulent  Nu of nanofluids can be predicted by traditional correlations and models. No abnormal heat transfer enhancement was observed. 
Kolade [37]  d_{p} = 4050 nm spherical Al_{2}O_{3}water rodlike carbon nanotubeoil  Tube/laminar  Nu is apparently larger than pure based fluid 
Duangthongsuk [14]  d_{p} = 21 nm spherical TiO_{2}water  Tube/turbulent  Pak and Cho (1998) correlation show better agreement to experimental data of Nu than Xuan and Li (2002) correlation 
Rea [96]  d_{p} = 50 nm spherical Al_{2}O_{3}water d_{p} = 50 nm spherical ZrO_{2}water  Tube/laminar  Nu of Al_{2}O_{3}water nanofluid show up to 27% more than pure water, ZrO_{2}water displays much lower enhancement. 
Jung [90]  d_{p} = 170 nm spherical Al_{2}O_{3}water d_{p} = 170 nm spherical Al_{2}O_{3}ethylene glycol  Rectangular microchannel/laminar  Nu increases with increasing the Reynolds number in laminar flow regime, appreciable enhancement of Nu is measured 
Heris [97]  spherical Al_{2}O_{3}water  Tube/laminar  Nu increases with increasing the Peclet number and φ, Brownian motion may play role in convective heat transfer enhancement 
Actually, "convective" k_{nf} values are not directly measured. Instead, wall temperature T_{w} and bulk temperature T_{b} are obtained and the heat transfer coefficient is then calculated as h = q_{w}/(T_{w}  T_{b}). From the definition of the Nusselt number, k_{nf} = hD/Nu where generally D is the hydraulic diameter. With h being basically measured and D known, either an analytic solution or an iterative numerical evaluation of Nu is required to calculate k_{nf}. Clearly, the accuracy of the "convective measurement method" largely depends on the degree of uncertainties related to the measured wall and bulk temperatures as well as the computed Nusselt number.
Optical measurement methods
In recent years, optical measurement methods have been proposed as noninvasive techniques for thermal conductivity measurements to improve accuracy [6–9, 13, 11, 27, 37]. Indeed, because the "hot wire" is a combination of heater and thermometer, interference is unavoidable. However, in optical techniques, detector and heater are always separated from each other, providing potentially more accurate data. Additionally, measurements are completed within several microseconds, i.e., much shorter than reported THWmeasurement times of 2 to 8 s, so that natural convection effects are avoided.
For example, Rusconi [6, 38] proposed a thermallensing (TL) measurement method to obtain k_{nf} data. The nanofluid sample was heated by a laserdiode module and the temperature difference was measured by photodiode as optical signals. After postprocessing, the thermal conductivity values were generated, which did not exceed meanfield theory results. Similar to the TL method, FRS have been used to investigate the thermal conductivity of welldispersed nanofluids [8, 39]. Again, their results did not show any anomalous enhancement either for Auor Al_{2}O_{3}nanofluids. Also, based on their data, no enhancement of thermal conductivity with temperature was observed. In contrast, Buongiorno et al. [9] presented data agreement when using both the THW method and FRS method. Another optical technique for thermal conductivity measurements of nanofluids is optical beam deflection [7, 40]. The nanofluid is heated by two parallel lines using a square current. The temperature change of nanofluids can be transformed to light signals captured by dual photodiodes. For Aunanofluids, Putnam [7] reported significantly lower k_{nf} enhancement than the data collected with the THW method.
However, other papers based on optical measurement techniques showed similar enhancement trends for nanofluid thermal conductivities as obtained with the thermal measurement methods. For example, Shaikh et al. [10] used the modern light flash technique (LFA 447) and measured the thermal conductivity of three types of nanofluids. They reported a maximum enhancement of 161% for the thermal conductivity of carbon nanotube (CNT)polyalphaolefin (PAO) suspensions. Such an enhancement is well above the prediction of the classical model by Hamilton and Crosser [41]. Also, Schmidt et al. [13] compared experimental data for Al_{2}O_{3}PAO and C_{10}H_{22}PAO nanofluids obtained via the Transient Optical Grating method and THW method. In both cases, the thermal conductivities were greater than expected from classical models. Additionally, Bazan [11] executed measurements by three different methods, i.e., laser flash (LF), transient plane source, and THW for PAObased nanofluids. They concluded that the THW method is the most accurate one while the LF method lacks precision when measuring nanofluids with low thermal conductivities. Also, no correlation between thermal conductivity and temperature was observed. Clearly, materials and experimental methods employed differ from study to study, where some of the new measurement methods were not verified repeatedly [6, 7]. Thus, it will be necessary for scientists to use different experimental techniques for the same nanofluids in order to achieve high comparable accuracy and prove reproducibility of the experimental results.
Experimental observations
Nearly all experimental results before 2005 indicate an anomalous enhancement of nanofluid thermal conductivity, assuming welldispersed nanoparticles. However, more recent efforts with refined transient hotwire and optical methods spawned a controversy on whether the anomalous enhancement beyond the meanfield theory is real or not. Eapen et al. [5] suggested a solution, arguing that even for dilute nanoparticle suspensions k_{nf} enhancement is a function of the aggregation state and hence connectivity of the particles; specifically, almost all experimental k_{nf} data published fall between lower and upper bounds predicted by classical theories.
In summary, k_{nf} is likely to improve with nanoparticle volume fraction and temperature as well as particle diameter, conductivity, and degree of aggregation, as further demonstrated in subsequent sections.
Thermal conductivity k_{nf}vs. volume fraction φ
Most experimental observations of nanofluids with just small nanoparticle volume fractions showed that k_{nf} will significantly increase when compared to the base fluid. For example, Lee and Choi [42] investigated CuOwater/ethylene glycol nanofluids with particle diameters 18.6 and 23.6 nm as well as Al_{2}O_{3}water/ethylene glycol nanofluids with particle diameters 24.4 and 38.4 nm and discovered a 20% thermal conductivity increase at a volume fraction of 4%. Wang [43] measured a 12% increase in k_{nf} for 28nmdiameter Al_{2}O_{3}water and 23 nm CuOwater nanofluids with 3% volume fraction. Li and Peterson [44] provided thermal conductivity expressions in terms of temperature (T) and volume fraction (φ) by using curve fitting for CuOwater and Al_{2}O_{3}water nanofluids. For nonmetallic particles, i.e., SiCwater nanofluids, Xie [45] showed a k_{nf} enhancement effect. Recently, Mintsa [26] provided new thermal conductivity expressions for Al_{2}O_{3}water and CuOwater nanofluids with particle sizes of 47, 36, and 29 nm by curve fitting their inhouse experimental data obtained by the THW method. Murshed [46] measured a 27% increase in 4% TiO_{2}water nanofluids with particle size 15 nm and 20% increase for Al_{2}O_{3}water nanofluids. However, Duangthongsuk [14] reported a more moderate increase of about 14% for TiO_{2}water nanofluids. Quite surprising, Moghadassi [47] observed a 50% increment of thermal conductivity for 5% CuOmonoethylene glycol (MEG) and CuOparaffin nanofluids.
Thermal conductivity k_{nf}vs. temperature T
Das [16] systematically discussed the relationship between thermal conductivity and temperature for nanofluids, noting significant increases of k_{nf} (T). More recently, Abareshi et al. [48] measured the thermal conductivity of Fe_{3}O_{4}water with the THW method and asserted that k_{nf} increases with temperature T. Indeed, from a theoretical (i.e., kinetics) viewpoint, with the increment of the nanofluid's bulk temperature T, molecules and nanoparticles are more active and able to transfer more energy from one location to another per unit time.
In contrast, many scientists using optical measurement techniques found no anomalous effective thermal conductivity enhancement when increasing the mixture temperature [[6–9, 29, 30, 37, 49], etc.]. Additionally, Tavman et al. [32] measured SiO_{2}water, TiO_{2}water, and Al_{2}O_{3}water by the 3ω method and claimed, without showing actual data points, that there is no anomalous thermal conductivity enhancement with increment of both volume fraction and temperature. Whether anomalous enhancement relationship between k_{nf} and temperature T exist or not is still open for debate.
Dependence of k_{nf}on other parameters
Potentially influential parameters on thermal conductivity, other than volume fraction and temperature, include pH value, type of base fluid, nanoparticle shape, degree of nanoparticle dispersion/interaction, and various additives. For example, Zhu et al. [50] showed that the pH of a nanofluid strongly affects the thermal conductivity of suspensions. Indeed, pH value influence the stability of nanoparticle suspensions and the charges of the particle surface thereby affect the nanofluid thermal conductivity. For pH equal to 8.09.0, the thermal conductivity of nanofluid is higher than other situations [50] Of the most common base fluids, water exhibits a higher thermal conductivity when compared to ethylene glycol (EG) for the same nanoparticle volume fraction [43, 44, 51–53]. However, thermal conductivity enhancement of EGbased nanofluids is stronger than for waterbased nanofluids [42, 43]. Different particle shapes may also influence the thermal conductivity of nanofluids. Nanoparticles with high aspect ratios seem to enhance the thermal conductivity further. For example, spherical particles show slightly less enhancement than those containing nanorods [54], while the thermal conductivity of CuOwaterbased nanofluids containing shuttlelikeshaped CuO nanoparticles is larger than those for CuO nanofluids containing nearly spherical CuO nanoparticles [55]. Another parameter influencing nanofluid thermal conductivity is particle diameter. Das [16], Patel [56] and Chon [57] showed the inverse dependence of particle size on thermal conductivity enhancement, considering three sizes of alumina nanoparticles suspended in water. Beck et al. [58] and Moghadassi et al. [47] reported that the thermal conductivity will increase with the decrease of nanoparticle diameters. However, Timofeeva et al. [53] reported that k_{nf} increases with the increment of nanoparticle diameter for SiCwater nanofluids without publishing any data. Other factors which may influence the thermal conductivity of nanofluids are sonification time [32] and/or surfactant mass fraction [32] to obtain welldispersed nanoparticles.
For other new experimental data, Wei X. et al. [59] reported nonlinear correlation between k_{nf} and synthesis parameters of nanoparticles as well as temperature T. Li and Peterson [60] showed natural convection deterioration with increase in nanoparticle volume fraction. This may be because the nanoparticle's Brownian motion smoothen the temperature gradient leading to the delay of the onset of natural convection. Also, higher viscosity of nanofluids can also induce such an effect. Wei et al. [61] claimed that the measured apparent thermal conductivity show timedependent characteristics within 15 min when using the THW method. They suggested that measurements should be made after 15 min in order to obtain accurate data. Chiesa et al. [23] investigated the impact of the THW apparatus orientation on thermal conductivity measurements; however, that aspect was found not to be significant. Shalkevich et al. [62] reported no abnormal thermal conductivity enhancement for 0.11% and 0.00055% of gold nanoparticle suspensions, which are rather low volume fractions. Beck et al. [63] and Teng et al. [15] provided curvefitted results based on their inhouse experimental data, reflecting correlations between k_{nf} and several parameters, i.e., volume fraction, bulk temperature and particle size. Both models are easy to use for certain types of nanofluids. Ali et al. [27] proposed hot wirelaser probe beam method to measure nanofluid thermal conductivity and confirmed that particle clustering has a significant effect on thermal conductivity enhancement.
Theoretical studies
Significant differences among published experimental data sets clearly indicate that some findings were inaccurate. Theoretical analyses, mathematical models, and associated computer simulations may provide additional physical insight which helps to explain possibly anomalous enhancement of the thermal conductivity of nanofluids.
Classical models
Classical models for effective thermal conductivity of mixtures
Dynamical models and comparisons with experimental data
When using the classical models, it is implied that the nanoparticles are stationary to the base fluid. In contrast, dynamic models are taking the effect of the nanoparticles' random motion into account, leading to a "micromixing" effect [70]. In general, anomalous thermal conductivity enhancement of nanofluids may be due to:

Brownianmotioninduced micromixing;

heatresistance lowering liquidmolecule layering at the particle surface;

higher heat conduction in metallic nanoparticles;

preferred conduction pathway as a function of nanoparticle shape, e.g., for carbon nanotubes;

augmented conduction due to nanoparticle clustering.
Up front, while the impact of microscale mixing due to Brownian motion is still being debated, the effects of nanoparticle clustering and preferred conduction pathways also require further studies.
Oezerinc et al. [71] systematically reviewed existing heat transfer mechanisms which can be categorized into conduction, nanoscale convection and/or nearfield radiation [22], thermal waves propagation [67, 72], quantum mechanics [73], and local thermal nonequilibrium [74].
For a better understanding of the micromixing effect due to Brownian motion, the works by Leal [75] and Gupte [76] are of interest. Starting with the paper by Koo and Kleinstreuer [70], several models stressing the Brownian motion effect have been published [22]. Nevertheless, that effect leading to micromixing was dismissed by several authors. For example, Wang [43] compared Brownian particle diffusion time scale and heat transfer time scale and declared that the effective thermal conductivity enhancement due to Brownian motion (including particle rotation) is unimportant. Keblinski [77] concluded that the heat transferred by nanoparticle diffusion contributes little to thermal conductivity enhancement. However, Wang [43] and Keblinski [77] failed to consider the surrounding fluid motion induced by the Brownian particles.
Kumar [83] proposed a "moving nanoparticle" model, where the effective thermal conductivity relates to the average particle velocity which is determined by the mixture temperature. However, the solidfluid interaction effect was not taken into account.
Summary and future work
Nanofluids, i.e., welldispersed metallic nanoparticles at low volume fractions in liquids, enhance the mixture's thermal conductivity over the basefluid values. Thus, they are potentially useful for advanced cooling of microsystems. Still, key questions linger concerning the best nanoparticleandliquid pairing and conditioning, reliable measurements of achievable k_{nf} values, and easytouse, physically sound computer models which fully describe the particle dynamics and heat transfer of nanofluids. At present, experimental data and measurement methods are lacking consistency. In fact, debates are still going on whether the anomalous enhancement is real or not, and what are repeatable correlations between k_{nf} and temperature, nanoparticle size/shape, and aggregation state. Clearly, additional benchmark experiments are needed, using the same nanofluids subject to different measurement methods as well as variations in nanofluid characteristics. This would validate new, minimally intrusive techniques and verify the reproducibility of experimental results.
Concerning theories/correlations which try to explain thermal conductivity enhancement for all nanofluids, not a single model can predict a wide range of experimental observations. However, many experimental data sets may fit between the lower and upper meanfield bounds originally proposed by Maxwell [1], where the static nanoparticle configurations may range between the two extremes of a dispersed phase to a continuous phase. Dynamic k_{nf} models postulate an enhancement above the classic Maxwell theory and thereby provide additional physical insight. Clearly, it will be necessary to consider not only one possible mechanism but combine several mechanisms and compare predictive results to new benchmark experimental data sets.
Notes
Declarations
Authors’ Affiliations
References
 Maxwell JC: A Treatise on Electricity and Magnetism. Oxford: Clarendon; 1891.Google Scholar
 Masuda H, Ebata A, Teramea K, Hishinuma N: Alteration of thermal conductivity and viscosity of liquid by dispersing ultrafine particles. Netsu Bussei 1993, 4: 227–233.View ArticleGoogle Scholar
 Eastman JA, Choi US, Li S, Thompson LJ, Lee S: Enhanced thermal conductivity through the development of nanofluids. In Nanophase and Nanocomposite Materials II. Edited by: Komarneni S, Parker JC, Wollenberger HJ. Pittsburg: Materials Research Society; 1997:3–11.Google Scholar
 Yu WH, France DM, Routbort JL, Choi SUS: Review and comparison of nanofluid thermal conductivity and heat transfer enhancements. Heat Transfer Engineering 2009, 29: 432–460. 10.1080/01457630701850851View ArticleGoogle Scholar
 Eapen J, Rusconi R, Piazza R, Yip S: The classical nature of thermal conduction in nanofluids. Journal of Heat Transfer 2010., 132: 102402–1102402–14. 102402110240214. 10.1115/1.4001304Google Scholar
 Rusconi R, Rodari E, Piazza R: Optical measurements of the thermal properties of nanofluids. Applied Physics Letters 2006., 89: 261916–12619163. 26191612619163. 10.1063/1.2425015Google Scholar
 Putnam SA, Cahill DG, Braun PV: Thermal conductivity of nanoparticle suspensions. Journal of Applied Physics 2006., 99: 084308–1084308–6. 08430810843086. 10.1063/1.2189933Google Scholar
 Venerus DC, Kabadi MS, Lee S, PerezLuna V: Study of thermal transport in nanoparticle suspensions using forced Rayleigh scattering. Journal of Applied Physics 2006., 100: 094310–1094310–5. 09431010943105. 10.1063/1.2360378Google Scholar
 Buongiorno J, Venerus DC, Prabhat N: A benchmark study on the thermal conductivity of nanofluids. Journal of Applied Physics 2009., 106: 094312–1094312–14. 094312109431214. 10.1063/1.3245330Google Scholar
 Shaikh S, Lafdi K: Thermal conductivity improvement in carbon nanoparticle doped PAO oil: An Experimental Study. Journal of Applied Physics 101: 064302–1064302–7. 06430210643027.Google Scholar
 Bazan JAN: Thermal conductivity of polyaelphaolefin (PAO)based nanofluids. Ph.D. Thesis, University of Dayton, Dayton, OH, USA. 2010.Google Scholar
 Yoo DH, Hong KS, Yang HS: Study of thermal conductivity of nanofluids for the application of heat transfer fluids. Thermochim Acta 2007, 455.Google Scholar
 Schmidt AJ, Chiesa M, Torchinsky DH, Johnson JA, Nelson KA, Chen G: Thermal conductivity of nanoparticle suspension in insulating media measured with a transient optical grating and a hotwire. Journal of Applied Physics 2008., 103: 083529–1083529–5. 08352910835295.Google Scholar
 Duangthongsuk W, Wongwises S: Measurement of temperaturedependent thermal conductivity and viscosity of TiO_{2}water nanofluids. Experimental Thermal and Fluid Science 2009, 33: 706–714. 10.1016/j.expthermflusci.2009.01.005View ArticleGoogle Scholar
 Teng TP, Hung YH, Teng TC, Mo HE, Hsu HG: The effect of alumina/water nanofluid particle size on thermal conductivity. Applied Thermal Engineering 2010, 30: 2213–2218. 10.1016/j.applthermaleng.2010.05.036View ArticleGoogle Scholar
 Das SK, Putra N, Theisen P, Roetzel W: Temperature dependence of thermal conductivity enhancement for nanofluids. Journal of Heat Transfer 2003, 125: 567–574. 10.1115/1.1571080View ArticleGoogle Scholar
 Czarnetzki W, Roetzel W: Temperature oscillation techniques for simultaneous measurement of thermal diffusivitiy and conductivity. International Journal of Thermophysics 1995, 16: 413–422. 10.1007/BF01441907View ArticleGoogle Scholar
 Choi TY, Maneshian MH: Measurement of the thermal conductivity of a waterbased singlewall carbon nanotube colloidal suspension with a modified 3w method. Nanotechnology 2009., 20: 315706–1315706–6. 31570613157066.Google Scholar
 Paul G, Chopkar M, Manna I, Das PK: Techniques for measuring the thermal conductivity of nanofluids: a review. Renewable and Sustainable Energy Reviews 2010, 14: 1913–1924. 10.1016/j.rser.2010.03.017View ArticleGoogle Scholar
 Feng Y: A new thermal conductivity model for nanofluids with convection heat transfer application. MS thesis, North Carolina State University, Raleigh, NC, USA. 2010.Google Scholar
 Vadasz P: Rendering the transient hot wire experimental method for thermal conductivity estimation to twophase systemstheoretical leading order results. Journal of Heat Transfer 2010., 132: 081601–1081601–7. 08160110816017.Google Scholar
 Das SK, Choi SUS, Yu W, Pradeep T: Nanofluids: Science and Technology. New Jersey: Wiley; 2008.Google Scholar
 Chiesa M, Simonsen AJ: The importance of suspension stability for hotwire measurements of thermal conductivity of colloidal suspensions. 16th Australasian Fluid Mechanics Conference, Gold Coast, Australia 2010.Google Scholar
 Zhang X, Gu H, Fujii M: Experimental study on the effective thermal conductivity and thermal diffusivity of nanofluid. AIAA Journal 2006, 41: 831–840. 10.2514/2.2044View ArticleGoogle Scholar
 Woodfield PL: A twodimensional analytical solution for the transient shorthotwire method. International Journal of Thermophysics 2008, 29: 1278–1298. 10.1007/s107650080469yView ArticleGoogle Scholar
 Mintsa HA, Roy G, Nguyen CT, Doucet D: New temperature dependent thermal conductivity data for waterbased nanofluids. International Journal of Thermal Sciences 2009, 48: 363–371. 10.1016/j.ijthermalsci.2008.03.009View ArticleGoogle Scholar
 Ali FM, Yunus WMM, Moksin MM, Talib ZA: The effect of volume fraction concentration on the thermal conductivity and thermal diffusivity of nanofluids: numerical and experimental. Review of Scientific Instruments 2010., 81: 074901–1074901–9. 07490110749019. 10.1063/1.3458011Google Scholar
 Patel HE, Sundararajan T, Das SK: An experimental investigation into the thermal conductivity enhancement in oxide and metallic nanofluids. Journal of Nanoparticle Research 2010, 12: 1015–1031. 10.1007/s1105100996582View ArticleGoogle Scholar
 Ju YS, Kim J, Hung MT: Experimental study of heat conduction in aqueous suspensions of aluminum oxide nanoparticles. Journal of Heat Transfer 2008., 130: 092403–1092403–6. 09240310924036.Google Scholar
 Li CH, Williams W: Transient and steadystate experimental comparison study of effective thermal conductivity of Al_{2}O_{3}water nanofluids. Journal of Heat Transfer 2008., 130: 042407–1042407–7. 04240710424077.Google Scholar
 Turgut A, Tavman I, Chirtoc M, Schuchmann HP, Sauter C, Tavman S: Thermal conductivity and viscosity measurements of waterbased TiO2 nanofluids. International Journal of Thermophysics 2009, 30: 1213–1226. 10.1007/s1076500905942View ArticleGoogle Scholar
 Tavman I, Turgut A: An investigation on thermal conductivity and viscosity of water based nanofluids. Microfluidics Based Microsystems 2010, 0: 139–162. full_textView ArticleGoogle Scholar
 Iygengar AS, Abramson AR: Comparative radial heat flow method for thermal conductivity measurement of liquids. Journal of Heat Transfer 2009., 131: 064502–1064502–3. 06450210645023.Google Scholar
 Kusiak A, Pradere C, Battaglia JL: Measuring the thermal conductivity of liquids using photothermal radiometry. Measurement Science and Technology 2010., 21: 015403–1015403–6. 01540310154036. 10.1088/09570233/21/1/015403Google Scholar
 Rousan AA, Roy DM: A thermal comparator method for measuring thermal conductivity of cementitious materials. Industrial and Engineering Chemistry Product Research and Development 1983, 22: 349–351. 10.1021/i300010a035View ArticleGoogle Scholar
 Lee JH: Convection Performance of Nanofluids for Electronics Cooling, Ph. D. Dissertation. Stanford University, CA, USA; 2009.Google Scholar
 Kolade B, Goodson KE, Eaton JK: Convective performance of nanofluids in a laminar thermally developing tube flow. Journal of Heat Transfer 2009., 131: 052402–1052402–8. 05240210524028. 10.1115/1.3013831Google Scholar
 Rusconi R, Isa L, Piazza R: Thermallensing measurement of particle thermophoresis in aqueous dispersions. Journal of Optical Society of America 2004, 21(3):605–616. 10.1364/JOSAB.21.000605View ArticleGoogle Scholar
 Venerus DC, Schieber JD, Iddir H, Guzman JD, Broerman AW: Measurement of thermal diffusivity in polymer melts using forced rayleigh light scattering. Journal of Polymer Science: Part B: Polymer Physics 1999, 37: 1069–1078. 10.1002/(SICI)10990488(19990601)37:11<1069::AIDPOLB3>3.0.CO;2UView ArticleGoogle Scholar
 Putnam SA, Cahill DG: Micronscale apparatus for measurements of thermodiffusion in liquids. Review of Scientific Instruments 2004, 75(7):2368–2372. 10.1063/1.1765761View ArticleGoogle Scholar
 Hamilton RL, Crosser OK: Thermal conductivity of heterogeneous twocomponent systems. Industrial Engineering and Chemistry Fundamentals 1962, 1(3):187–191. 10.1021/i160003a005View ArticleGoogle Scholar
 Lee S, Choi SUS: Measuring thermal conductivity of fluids containing oxide nanoparticles. Journal of Heat Transfer 1999, 121: 280–289. 10.1115/1.2825978View ArticleGoogle Scholar
 Wang XW, Xu XF, Choi SUS: Thermal conductivity of nanoparticlefluid mixture. Journal of Thermalphysics and Heat Transfer 1999, 13: 474–480. 10.2514/2.6486View ArticleGoogle Scholar
 Li CH, Peterson GP: Experimental investigation of temperature and volume fraction variations on the effective thermal conductivity of nanoparticle suspensions (nanofluids). Journal of Applied Physics 2006, 99(8):084314. 10.1063/1.2191571View ArticleGoogle Scholar
 Xie H, Wang J, Xi T, Liu Y: Thermal conductivity of suspensions containing nanosized SiC particles. International Journal of Thermophysics 2002, 23(2):571–580. 10.1023/A:1015121805842View ArticleGoogle Scholar
 Murshed SMS, Leong KC, Yang C: A combined model for the effective thermal conductivity of nanofluids. Applied Thermal Engineering 2009, 29: 2477–2483. 10.1016/j.applthermaleng.2008.12.018View ArticleGoogle Scholar
 Moghadassi AR, Hosseini SM, Henneke DE: Effect of CuO nanoparticles in enhancing the thermal conductivities of monoethylene glycol and paraffin fluids. Industrial Engineering and Chemistry Research 2010, 49: 1900–1904. 10.1021/ie901060eView ArticleGoogle Scholar
 Abareshi M, Goharshiadi EK, Zebarjad SM, Fadafan HK, Youssefi A: Fabrication, characterization and measurement of thermal conductivity of Fe_{3}O_{4}nanofluids. Journal of Magnetism and Magnetic Materials 2010, 322(24):3895–3901. 10.1016/j.jmmm.2010.08.016View ArticleGoogle Scholar
 Williams W, Buongiorno J, Hu LW: Experimental investigation of turbulent convective heat transfer and pressure loss of alumina/water and zirconia/water nanoparticle colloids (nanofluids) in horizontal tubes. Journal of Heat Transfer 2008., 130: 042412–1042412–7. 04241210424127. 10.1115/1.2818775Google Scholar
 Zhu D, Li X, Wang N, Wang X, Gao J, Li H: Dispersion behavior and thermal conductivity characteristics of Al_{2}O_{3}H_{2}O nanofluids. Current Applied Physics 2009, 9: 131–139. 10.1016/j.cap.2007.12.008View ArticleGoogle Scholar
 Jang SP, Choi SUS: Role of Brownian motion in the enhanced thermal conductivity of nanofluids. Applied Physics Letters 2004, 84: 4316–4318. 10.1063/1.1756684View ArticleGoogle Scholar
 Timofeeva EV, Gavrilov AN, McCloskey JM, Tolmachev YV: Thermal conductivity and particle agglomeration in alumina nanofluids: experiment and theory. Physical Review E 2007., 76: 061203–1061203–16. 061203106120316. 10.1103/PhysRevE.76.061203Google Scholar
 Timofeeva EV, Smith DS, Yu W, France DM, Singh D, Routbort JL: Particle size and interfacial effects on thermophysical and heat transfer characteristics of waterbased alphaSiC nanofluids. Nanotechnology 2010., 21: 215703–1215703–10. 215703121570310. 10.1088/09574484/21/21/215703Google Scholar
 Murshed SMS, Leong KC, Yang C: Enhanced thermal conductivity of TiO2water based nanofluids. International Journal of Thermal Sciences 2005, 44: 367. 10.1016/j.ijthermalsci.2004.12.005View ArticleGoogle Scholar
 Zhu HT, Zhang CY, Tang YM, Wang JX: Novel synthesis and thermal conductivity of CuO nanofluid. Journal of Physical Chemistry C 2007, 111: 1646. 10.1021/jp065926tView ArticleGoogle Scholar
 Patel HE, Das SK, Sundararajan T, Sreekumanran NA, George B, Pradeep T: Thermal conductivities of naked and monolayer protected metal nanoparticle based nanofluids: manifestation of anomalous enhancement and chemical effects. Applied Physics Letters 2003, 83: 2931–2933. 10.1063/1.1602578View ArticleGoogle Scholar
 Chon CH, Kihm KD, Lee SP, Choi SUS: Empirical correlation finding the role of temperature and particle size for nanofluid (Al_{2}O_{3}) thermal conductivity enhancement. Applied Physics Letters 2005., 87: 153107–1153107–3. 15310711531073. 10.1063/1.2093936Google Scholar
 Beck MP, Yuan Y, Warrier P, Teja AS: The effect of particle size on the thermal conductivity of alumina nanofluids. Journal of Nanoparticle Research 2009, 11: 1129–1136. 10.1007/s1105100895002View ArticleGoogle Scholar
 Wei X, Kong T, Zhu H, Wang L: CuS/Cu_{2}S nanofluids: synthesis and thermal conductivity. International of Heat and Mass Transfer 2010, 53: 1841–1843. 10.1016/j.ijheatmasstransfer.2010.01.006View ArticleGoogle Scholar
 Li CH, Peterson GP: Experimental studies of natural convection heat transfer of Al_{2}O_{3}/DI water nanoparticle suspensions (nanofluids). Advances in Mechanical Engineering 2010., 2010: 742739–1742739–10. 742739174273910.Google Scholar
 Wei Y, Xie H, Chen L, Li Y: Investigation on the thermal transport properties of ethylene glycolbased nanofluids containing copper nanoparticles. Powder Technology 2010, 197: 218–221. 10.1016/j.powtec.2009.09.016View ArticleGoogle Scholar
 Shalkevich N, Escher W, Buergi T, Michel B, Ahmed L, Poulikakos D: On the thermal conductivity of gold nanoparticle colloid. Langmuir 2010, 26(2):663–670. 10.1021/la9022757View ArticleGoogle Scholar
 Beck MP, Yuan Y, Warrier P, Teja AS: The thermal conductivity of alumina nanofluids in water, ethylene glycol, and ethylene glycol + water mixture. Journal of Nanoparticles Research 2010, 12: 1469–1477. 10.1007/s1105100997169View ArticleGoogle Scholar
 Jeffrey DJ: Conduction through a random suspension of spheres. Proceedings of Royal Society, A 1973, 335: 355–367. 10.1098/rspa.1973.0130View ArticleGoogle Scholar
 Davis RH: The effective thermal conductivity of a composite material with spherical inclusions. International Journal of Thermophysics 1986, 7: 609–620. 10.1007/BF00502394View ArticleGoogle Scholar
 Bruggeman DAG: Berechnung verschiedener physikalischer konstanten von heterogenen substanzen, IDielektrizitatskonstanten und leitfahigkeiten der mischkorper aus isotropen substanzen. Annalen der Physik, Leipzig 1935, 24: 636–679. 10.1002/andp.19354160705View ArticleGoogle Scholar
 Wang LQ, Zhou XS, Wei XH: Heat conduction mathematical models and analytical solutions. Berlin: SpringerVerlag; 2008.Google Scholar
 Hashin Z, Shtrikman S: Conductivity of polycrystals. Physical Review 1963, 130: 129–133. 10.1103/PhysRev.130.129View ArticleGoogle Scholar
 Koo J, Kang Y, Kleinstreuer C: A nonlinear effective thermal conductivity model for carbon nanotube and nanofiber suspensions. Nanotechnology 2008., 19: 375705–1375705–7. 37570513757057.Google Scholar
 Koo J, Kleinstreuer C: A new thermal conductivity model for nanofluids. Journal of Nanoparticle Research 2004, 6: 577–588. 10.1007/s1105100431705View ArticleGoogle Scholar
 Oezerinc S, Kakac S, Yazicioglu AG: Enhanced thermal conductivity of nanofluids: A stateoftheart review. Microfluid Nanofluid 2010, 8: 145–170. 10.1007/s1040400905244View ArticleGoogle Scholar
 Wang LQ, Fan J: Nanofluids research: key issues. Nanoscale Research Letter 2010, 5: 1241–1252. 10.1007/s1167101096386View ArticleGoogle Scholar
 Prevenslik T: Nanoscale Heat Transfer by Quantum Mechanics. Fifth International Conference on Thermal Engineering: Theory and Applications, Marrakesh, Morocco 2010.Google Scholar
 Nield DA, Kuznetsov AV: The effect of local thermal nonequilibrium on the onset of convection in a nanofluid. Journal of Heat Transfer 2010., 132: 052405–1052405–7 05240510524057Google Scholar
 Leal LG: On the effective conductivity of a dilute suspension of spherical drops in the limit of low particle Peclet number. Chem Eng Commun 1973, 1: 21–31. 10.1080/00986447308960412View ArticleGoogle Scholar
 Gupte SK, Advani SG: Role of microconvection due to nonaffine motion of particles in a monodisperse suspension. Int J Heat Mass Transfer 1995, 38(16):2945–2958. 10.1016/00179310(95)00060MView ArticleGoogle Scholar
 Keblinski P, Phillpot SR, Choi SUS, Eastman JA: Mechanisms of heat flow in suspensions of nanossezed particles (nanofluids). International Journal of Heat and Mass Transfer 2002, 45: 855–863. 10.1016/S00179310(01)001752View ArticleGoogle Scholar
 Jang SP, Choi SUS: Effects of various parameters on nanofluid thermal conductivity. ASME J Heat Transfer 2007, 129: 617–623. 10.1115/1.2712475View ArticleGoogle Scholar
 Jang SP, Choi SUS: Cooling performance of a microchannel heat sink with nanofluids. Appl Therm Eng 2006, 26: 2457–2463. 10.1016/j.applthermaleng.2006.02.036View ArticleGoogle Scholar
 Kleinstreuer C, Li J: Discussion: effects of various parameters on nanofluid thermal conductivity. ASME Journal of Heat Transfer 2008., 130: 025501–1025501–3. 02550110255013. 10.1115/1.2812307Google Scholar
 Prasher R: Brownianmotionbased convectiveconductive model for the effective thermal conductivity of nanofluids. Journal of Heat Transfer 2006, 128: 588–595. 10.1115/1.2188509View ArticleGoogle Scholar
 Li J: Computational analysis of nanofluid flow in microchannels with applications to microheat sinks and bioMEMS, PhD Thesis. NC State University, Raleigh, NC, the United States; 2008.Google Scholar
 Kumar DH, Patel HE, Kumar VRR, Sundararajan T, Pradeep T, Das SK: Model for heat conduction in nanofluids. Physical Review Letters 2004., 93: 144301–1144301–4. 14430111443014. 10.1103/PhysRevLett.93.144301Google Scholar
 Koo JM: Computational nanofluid flow and heat transfer analyses applied to microsystems, Ph.D Thesis. NC State University, Raleigh, NC, USA; 2005.Google Scholar
 Bao Y: Thermal conductivity equations based on Brownian motion in suspensions of nanoparticles (nanofluids). Journal of Heat Transfer 130: 042408–1042408–5. 04240810424085.Google Scholar
 Feng Y, Kleinstreuer C: Nanofluid convective heat transfer in a paralleldisk system. International Journal of Heat and Mass Transfer 2010, 53: 4619–4628. 10.1016/j.ijheatmasstransfer.2010.06.031View ArticleGoogle Scholar
 Chopkar M, Sudarshan S, Das PK, Manna I: Effect of particle size on thermal conductivity of nanofluid. Metallurgical and Materials Transactions A 2008, 39A: 1535–1542. 10.1007/s1166100794447View ArticleGoogle Scholar
 Wu D, Zhu H, Wang L, Liu L: Critical issues in nanofluids preparation, characterization and thermal conductivity. Current Nanoscience 2009, 5: 103–112. 10.2174/157341309787314548View ArticleGoogle Scholar
 Singh D, Timofeeva E, Yu W, Routbort J, France D, Smith D, LopezCepero JM: An investigation of silicon carbidewater nanofluid for heat transfer applications. Journal of Applied Physics 2009., 15: 064306–1064306–6. 06430610643066.Google Scholar
 Jung YJ, Jung YY: Thermal conductivity enhancement of nanofluids in conjunction with electrical double layer (EDL). International Journal of Heat and Mass Transfer 2009, 52: 525–528. 10.1016/j.ijheatmasstransfer.2008.07.016View ArticleGoogle Scholar
 Pak BC, Cho YI: Hydrodynamic and heat transfer study of dispersed fluids with submicron metallic oxide particles. Exp Heat Transfer 1998, 11: 151–170. 10.1080/08916159808946559View ArticleGoogle Scholar
 Li Q, Xuan Y: Convective heat transfer and flow characteristics of Cuwater nanofluid. Science in China (Series E) 2002, 45: 408–416.Google Scholar
 Wen D, Ding Y: Experimental investigation into convective heat transfer of nanofluids at the entrance region under laminar flow conditions. International Journal of Heat and Mass Transfer 2004, 47: 5181–5188. 10.1016/j.ijheatmasstransfer.2004.07.012View ArticleGoogle Scholar
 Ding Y, Alias H, Wen D, Williams RA: Heat transfer of aqueous suspensions of carbon nanotubes (CNT nanofluids). International Journal of Heat and Mass Transfer 2006, 49: 240–250. 10.1016/j.ijheatmasstransfer.2005.07.009View ArticleGoogle Scholar
 Heris SZ, Esfahany MN, Etemad SG: Experimental investigation of convective heat transfer of Al_{2}O_{3}/water nanofluid in circular tube. International Journal of Heat and Fluid Flow 2007, 28: 203–210. 10.1016/j.ijheatfluidflow.2006.05.001View ArticleGoogle Scholar
 Rea U, McKrell T, Hu L, Buongiorno J: Laminar convective heat transfer and viscous pressure loss of aluminawater and zirconiawater nanofluids. International Journal of Heat and Mass Transfer 2009, 52: 2042–2048. 10.1016/j.ijheatmasstransfer.2008.10.025View ArticleGoogle Scholar
 Heris SZ, Etemad SGh, Esfahany MN: Convective heat transfer of a Cu/water nanofluid flowing through a circular tube. Experimental Heat Transfer 2009, 22: 217–227. 10.1080/08916150902950145View ArticleGoogle Scholar
Copyright
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.